Download (direct link):
it is these that experience different environments in the various triads.
If dyad information is sufficient, the resonances of the methylenes in
the chain backbone are measured. Structures [XIII] and [XIV] show that
these serve as probes of the environment in dyads.
Polymers with Microstructure
In the next section we shall examine in more detail how this type of
NMR data is interpreted.
7.11 Measuring Stereoregularity by Nuclear Magnetic Resonance
It is not the purpose of this book to discuss in detail the contributions
of NMR spectroscopy to the determination of molecular structure. This is
a specialized field in itself and a great deal has been written on the
subject. In this section we shall consider only the application of NMR to
the elucidation of stereoregularity in polymers. Numerous other
applications of this powerful technique have also been made in polymer
chemistry, including the study of positional and geometrical isomerism
(Sec. 1.6), copolymers (Sec. 7.7), and helix-coil transitions (Sec.
1.11). We shall also make no attempt to compare the NMR spectra of
various different polymers; instead, we shall examine only the NMR
spectra of different poly (methyl methacrylate) preparations to
illustrate the capabilities of the method, using the first system that
was investigated by this technique as the example.
Figure 7.10 shows the 60-MHz spectra of poly (methyl methacrylate)
prepared with different catalysts so that predominately isotactic,
syndiotactic, and atactic products are formed. The three spectra in Fig.
7.10 are identified in terms of this predominant character. It is
apparent that the spectra are quite different, especially in the range of
5 values between about 1 and 2 ppm. Since the atactic polymer has the
least regular structure, we concentrate on the other two to make the
assignment of the spectral features to the various protons.
Several observations from the last section provide the basis of
interpreting these spectra:
1. The hydrogens of the methylene group in the backbone of the poly
(methyl methacrylate) produce a single peak in a racemic dyad, as
illustrated by structure [XVI].
2. The same group of hydrogens in a meso dyad [XIII] produce a
of peaks: two different chemical shifts, each split into two by
hydrogens in the methylene.
3. The peaks centered at 5 = 1.84 ppm-a singlet in the syndiotactic and
a quartet in the isotactic polymers-are thus identified with these
protons. This provides an unambiguous identification of the predominant
stereoregularity of these samples.
4. The features that occur near 5 = 1.0 ppm are associated with the
protons of the a-methyl group. The location of this peak depends on the
configurations of the nearest neighbors.
5. Working from the methylene assignments, we see that the peak at
5 = 1.22
ppm in the isotactic polymer arises from the methyl in the
center of an
Measuring Stereoregularity by NMR
Figure 7.10 Nuclear magnetic resonance spectra of three poly(methyl
methacrylate samples. Curves are labeled according to the preominant
tacticity of samples. [From D. W. McCall and W. P. Slichter, in Newer
Methods of Polymer Characterization, B. Ke (Ed.), Interscience, New York,
1964, used with permission.]
isotactic triad, the peak at 5 = 0.87 ppm from a syndiotactic triad,
and the peak at 5 = 1.02 ppm from a homotactic triad.
6. The peak at 5 = 3.5 ppm is due to the ester methoxy group.
Polymers with Microstructure
Once these assignments are made, the areas under the various peaks
can be measured to determine the various fractions:
1. The area under the methylene peaks is proportional to the dyad
concentration: The singlet gives the racemic dyads and the quartet gives
the meso dyads.
2. The area under one of the methyl peaks is proportional to the
concentration of the corresponding triad.
3. It is apparent that it is not particularly easy to determine the
exact areas of these features when the various contributions occur
together to any significant extent. This is clear from the atactic
spectrum, in which slight shoulders on both the methylene and methyl
peaks are the only evidence of meso methylenes and iso methyls.
The spectra shown in Fig. 7.10 were early attempts at this kind of
experiment, and the measurement of peak areas in this case was a rather
subjective affair. We shall continue with an analysis of these spectra-
subjectivity and alleven though improved instrumentation has resulted in
much improved spectra. One development that has produced better
resolution in spectra is the use of higher magnetic fields. As the
magnetic field increases, the chemical shifts for the various features
are displaced proportionately. The splitting caused by spin-spin
coupling, on the other hand, is unaffected. This can produce a